# Electronic Supplementary Material (ESI) for Journal of Materials Chemistry C.
# This journal is © The Royal Society of Chemistry 2023

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_database_code_depnum_ccdc_archive 'CCDC 2217264'
loop_
_audit_author_name
_audit_author_address
'Zhaowei Hu'
;Shanghai Institute of Technology
China
;
_audit_update_record             
;
2022-11-03 deposited with the CCDC.	2023-02-02 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        Na3Rb6(CO3)3(NO3)2Br.6H2O
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C3 H12 Br N2 Na3 O21 Rb6'
_chemical_formula_weight         1073.85

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Br Br -0.2901 2.4595 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_H-M   'P 63/m c m'

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'x-y, x, z+1/2'
'-y, x-y, z'
'-x, -y, z+1/2'
'-x+y, -x, z'
'y, -x+y, z+1/2'
'-y, -x, -z'
'x-y, -y, -z+1/2'
'x, x-y, -z'
'y, x, -z+1/2'
'-x+y, y, -z'
'-x, -x+y, -z+1/2'
'-x, -y, -z'
'-x+y, -x, -z-1/2'
'y, -x+y, -z'
'x, y, -z-1/2'
'x-y, x, -z'
'-y, x-y, -z-1/2'
'y, x, z'
'-x+y, y, z-1/2'
'-x, -x+y, z'
'-y, -x, z-1/2'
'x-y, -y, z'
'x, x-y, z-1/2'

_cell_length_a                   9.6086(4)
_cell_length_b                   9.6086(4)
_cell_length_c                   15.8641(15)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_volume                     1268.43(14)
_cell_formula_units_Z            2
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    4890
_cell_measurement_theta_min      2.4476
_cell_measurement_theta_max      28.2582

_exptl_crystal_description       block
_exptl_crystal_colour            ?
_exptl_crystal_size_max          ?
_exptl_crystal_size_mid          ?
_exptl_crystal_size_min          ?
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.812
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1004
_exptl_absorpt_coefficient_mu    13.199
_exptl_absorpt_correction_type   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_process_details   ?

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            11287
_diffrn_reflns_av_R_equivalents  0.0466
_diffrn_reflns_av_sigmaI/netI    0.0173
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_theta_min         2.57
_diffrn_reflns_theta_max         28.28
_reflns_number_total             603
_reflns_number_gt                583
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0000P)²+6.1761P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    mixed
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.0008(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         603
_refine_ls_number_parameters     40
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0344
_refine_ls_R_factor_gt           0.0327
_refine_ls_wR_factor_ref         0.0696
_refine_ls_wR_factor_gt          0.0691
_refine_ls_goodness_of_fit_ref   1.345
_refine_ls_restrained_S_all      1.345
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Rb1 Rb 0.28581(6) 0.28581(6) 0.12021(3) 0.0309(2) Uani 1 2 d S . .
Na1 Na 0.3776(4) 0.0000 0.2500 0.0336(8) Uani 1 4 d S . .
N1 N 0.6667 0.3333 0.2500 0.0211(15) Uani 1 6 d S . .
C1 C 0.0000 0.0000 0.2500 0.018(2) Uani 1 12 d S . .
C2 C 0.6667 0.3333 0.0000 0.0213(18) Uani 1 6 d S . .
O1 O 0.6036(4) 0.6036(4) 0.1052(2) 0.0303(9) Uani 1 2 d S . .
H1 H 0.6456 0.5613 0.0705 0.045 Uiso 1 1 d R . .
O2 O 0.1333(4) 0.0000(4) 0.2500(2) 0.0328(14) Uani 1 4 d SR . .
O3 O 0.5122(5) 0.2561(2) 0.0000 0.0306(9) Uani 1 2 d S . .
O4 O 0.5252(5) 0.3076(5) 0.2500 0.0321(10) Uani 1 2 d S . .
Br1 Br 0.0000 0.0000 0.0000 0.0310(4) Uani 1 12 d S . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Rb1 O3 3.012(2) 17 ?
Rb1 O3 3.012(2) . ?
Rb1 O4 3.015(3) . ?
Rb1 O4 3.015(3) 19 ?
Rb1 O1 3.062(4) . ?
Rb1 O2 3.147(4) 3 ?
Rb1 O2 3.147(4) . ?
Rb1 Br1 3.3435(6) . ?
Rb1 O1 3.413(3) 3_655 ?
Rb1 O1 3.413(3) 5_565 ?
Rb1 Na1 3.834(3) 14_666 ?
Rb1 Na1 3.871(2) 3 ?
Rb1 H1 3.2294 . ?
Na1 O1 2.303(4) 18_656 ?
Na1 O1 2.303(4) 3_655 ?
Na1 O2 2.347(4) . ?
Na1 O4 2.560(4) 8 ?
Na1 O4 2.560(4) . ?
Na1 O4 2.683(5) 3_655 ?
Na1 O4 2.683(5) 21_655 ?
Na1 N1 3.0127(14) 19_545 ?
Na1 Rb1 3.834(3) 18_656 ?
Na1 Rb1 3.834(3) 3_655 ?
Na1 Rb1 3.871(2) 5 ?
Na1 Rb1 3.871(2) 16_556 ?
N1 O4 1.254(4) 3_655 ?
N1 O4 1.254(4) 14_666 ?
N1 O4 1.254(4) . ?
N1 Na1 3.0127(14) 3_655 ?
N1 Na1 3.0127(14) 14_666 ?
C1 O2 1.281(2) 14_556 ?
C1 O2 1.281(2) 3 ?
C1 O2 1.281(2) . ?
C1 Rb1 3.4324(6) 16_556 ?
C1 Rb1 3.4324(6) 5 ?
C1 Rb1 3.4324(6) 3 ?
C1 Rb1 3.4324(6) 14_556 ?
C1 Rb1 3.4324(6) 18_556 ?
C2 O3 1.285(4) 3_655 ?
C2 O3 1.285(4) 5_665 ?
C2 O3 1.285(4) . ?
O1 Na1 2.303(4) 14_666 ?
O1 Rb1 3.413(3) 3_665 ?
O1 Rb1 3.413(3) 5_665 ?
O1 H1 0.8918 . ?
O2 Rb1 3.147(4) 16_556 ?
O2 Rb1 3.147(4) 5 ?
O2 Rb1 3.147(4) 14_556 ?
O3 Rb1 3.012(2) 15 ?
O4 Na1 2.683(5) 14_666 ?
O4 Rb1 3.015(3) 16_556 ?
Br1 Rb1 3.3435(6) 13 ?
Br1 Rb1 3.3435(6) 17 ?
Br1 Rb1 3.3435(6) 3 ?
Br1 Rb1 3.3435(6) 15 ?
Br1 Rb1 3.3435(6) 5 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O3 Rb1 O3 90.08(2) 17 . ?
O3 Rb1 O4 136.61(10) 17 . ?
O3 Rb1 O4 82.92(7) . . ?
O3 Rb1 O4 82.92(7) 17 19 ?
O3 Rb1 O4 136.61(10) . 19 ?
O4 Rb1 O4 73.82(14) . 19 ?
O3 Rb1 O1 68.78(7) 17 . ?
O3 Rb1 O1 68.78(7) . . ?
O4 Rb1 O1 68.78(10) . . ?
O4 Rb1 O1 68.78(10) 19 . ?
O3 Rb1 O2 112.01(6) 17 3 ?
O3 Rb1 O2 150.88(5) . 3 ?
O4 Rb1 O2 92.49(9) . 3 ?
O4 Rb1 O2 67.66(8) 19 3 ?
O1 Rb1 O2 135.87(10) . 3 ?
O3 Rb1 O2 150.88(5) 17 . ?
O3 Rb1 O2 112.01(3) . . ?
O4 Rb1 O2 67.66(10) . . ?
O4 Rb1 O2 92.49(8) 19 . ?
O1 Rb1 O2 135.87(12) . . ?
O2 Rb1 O2 41.29(8) 3 . ?
O3 Rb1 Br1 84.07(6) 17 . ?
O3 Rb1 Br1 84.07(6) . . ?
O4 Rb1 Br1 136.99(9) . . ?
O4 Rb1 Br1 136.99(9) 19 . ?
O1 Rb1 Br1 140.78(8) . . ?
O2 Rb1 Br1 79.84(6) 3 . ?
O2 Rb1 Br1 79.84(7) . . ?
O3 Rb1 O1 135.83(7) 17 3_655 ?
O3 Rb1 O1 49.41(6) . 3_655 ?
O4 Rb1 O1 64.51(10) . 3_655 ?
O4 Rb1 O1 136.94(9) 19 3_655 ?
O1 Rb1 O1 103.92(5) . 3_655 ?
O2 Rb1 O1 102.78(5) 3 3_655 ?
O2 Rb1 O1 62.59(4) . 3_655 ?
Br1 Rb1 O1 75.98(6) . 3_655 ?
O3 Rb1 O1 49.41(6) 17 5_565 ?
O3 Rb1 O1 135.83(7) . 5_565 ?
O4 Rb1 O1 136.94(9) . 5_565 ?
O4 Rb1 O1 64.51(10) 19 5_565 ?
O1 Rb1 O1 103.92(5) . 5_565 ?
O2 Rb1 O1 62.59(8) 3 5_565 ?
O2 Rb1 O1 102.78(5) . 5_565 ?
Br1 Rb1 O1 75.98(6) . 5_565 ?
O1 Rb1 O1 150.31(10) 3_655 5_565 ?
O3 Rb1 Na1 94.32(6) 17 14_666 ?
O3 Rb1 Na1 94.32(6) . 14_666 ?
O4 Rb1 Na1 44.14(9) . 14_666 ?
O4 Rb1 Na1 44.14(9) 19 14_666 ?
O1 Rb1 Na1 36.93(8) . 14_666 ?
O2 Rb1 Na1 102.30(6) 3 14_666 ?
O2 Rb1 Na1 102.30(8) . 14_666 ?
Br1 Rb1 Na1 177.71(4) . 14_666 ?
O1 Rb1 Na1 104.21(6) 3_655 14_666 ?
O1 Rb1 Na1 104.21(6) 5_565 14_666 ?
O3 Rb1 Na1 80.67(4) 17 3 ?
O3 Rb1 Na1 170.67(4) . 3 ?
O4 Rb1 Na1 102.97(6) . 3 ?
O4 Rb1 Na1 41.36(9) 19 3 ?
O1 Rb1 Na1 106.34(5) . 3 ?
O2 Rb1 Na1 37.31(6) 3 3 ?
O2 Rb1 Na1 77.12(5) . 3 ?
Br1 Rb1 Na1 96.06(2) . 3 ?
O1 Rb1 Na1 139.67(7) 3_655 3 ?
O1 Rb1 Na1 36.19(7) 5_565 3 ?
Na1 Rb1 Na1 85.26(4) 14_666 3 ?
O3 Rb1 H1 72.7 17 . ?
O3 Rb1 H1 52.8 . . ?
O4 Rb1 H1 69.1 . . ?
O4 Rb1 H1 84.5 19 . ?
O1 Rb1 H1 16.0 . . ?
O2 Rb1 H1 150.3 3 . ?
O2 Rb1 H1 135.7 . . ?
Br1 Rb1 H1 129.6 . . ?
O1 Rb1 H1 90.4 3_655 . ?
O1 Rb1 H1 115.2 5_565 . ?
Na1 Rb1 H1 48.2 14_666 . ?
Na1 Rb1 H1 122.3 3 . ?
O1 Na1 O1 171.0(3) 18_656 3_655 ?
O1 Na1 O2 94.50(16) 18_656 . ?
O1 Na1 O2 94.50(17) 3_655 . ?
O1 Na1 O4 90.105(9) 18_656 8 ?
O1 Na1 O4 90.105(9) 3_655 8 ?
O2 Na1 O4 88.66(15) . 8 ?
O1 Na1 O4 90.105(9) 18_656 . ?
O1 Na1 O4 90.105(9) 3_655 . ?
O2 Na1 O4 88.66(15) . . ?
O4 Na1 O4 177.3(2) 8 . ?
O1 Na1 O4 86.68(10) 18_656 3_655 ?
O1 Na1 O4 86.68(10) 3_655 3_655 ?
O2 Na1 O4 137.54(13) . 3_655 ?
O4 Na1 O4 133.79(14) 8 3_655 ?
O4 Na1 O4 48.88(17) . 3_655 ?
O1 Na1 O4 86.68(10) 18_656 21_655 ?
O1 Na1 O4 86.68(10) 3_655 21_655 ?
O2 Na1 O4 137.54(13) . 21_655 ?
O4 Na1 O4 48.88(17) 8 21_655 ?
O4 Na1 O4 133.79(14) . 21_655 ?
O4 Na1 O4 84.91(19) 3_655 21_655 ?
O1 Na1 N1 88.24(6) 18_656 19_545 ?
O1 Na1 N1 88.24(6) 3_655 19_545 ?
O2 Na1 N1 112.97(10) . 19_545 ?
O4 Na1 N1 24.31(9) 8 19_545 ?
O4 Na1 N1 158.36(18) . 19_545 ?
O4 Na1 N1 109.48(13) 3_655 19_545 ?
O4 Na1 N1 24.57(8) 21_655 19_545 ?
O1 Na1 Rb1 53.01(12) 18_656 18_656 ?
O1 Na1 Rb1 117.98(16) 3_655 18_656 ?
O2 Na1 Rb1 147.52(10) . 18_656 ?
O4 Na1 Rb1 91.13(10) 8 18_656 ?
O4 Na1 Rb1 91.13(10) . 18_656 ?
O4 Na1 Rb1 51.51(8) 3_655 18_656 ?
O4 Na1 Rb1 51.51(8) 21_655 18_656 ?
N1 Na1 Rb1 70.78(6) 19_545 18_656 ?
O1 Na1 Rb1 117.98(16) 18_656 3_655 ?
O1 Na1 Rb1 53.01(12) 3_655 3_655 ?
O2 Na1 Rb1 147.52(10) . 3_655 ?
O4 Na1 Rb1 91.13(10) 8 3_655 ?
O4 Na1 Rb1 91.13(10) . 3_655 ?
O4 Na1 Rb1 51.51(8) 3_655 3_655 ?
O4 Na1 Rb1 51.51(8) 21_655 3_655 ?
N1 Na1 Rb1 70.78(6) 19_545 3_655 ?
Rb1 Na1 Rb1 64.97(6) 18_656 3_655 ?
O1 Na1 Rb1 125.17(10) 18_656 5 ?
O1 Na1 Rb1 61.02(8) 3_655 5 ?
O2 Na1 Rb1 54.36(10) . 5 ?
O4 Na1 Rb1 51.11(8) 8 5 ?
O4 Na1 Rb1 126.92(11) . 5 ?
O4 Na1 Rb1 147.63(3) 3_655 5 ?
O4 Na1 Rb1 90.86(7) 21_655 5 ?
N1 Na1 Rb1 70.23(2) 19_545 5 ?
Rb1 Na1 Rb1 141.00(4) 18_656 5 ?
Rb1 Na1 Rb1 101.88(2) 3_655 5 ?
O1 Na1 Rb1 61.02(8) 18_656 16_556 ?
O1 Na1 Rb1 125.17(10) 3_655 16_556 ?
O2 Na1 Rb1 54.36(10) . 16_556 ?
O4 Na1 Rb1 126.92(11) 8 16_556 ?
O4 Na1 Rb1 51.11(8) . 16_556 ?
O4 Na1 Rb1 90.86(7) 3_655 16_556 ?
O4 Na1 Rb1 147.63(3) 21_655 16_556 ?
N1 Na1 Rb1 142.48(4) 19_545 16_556 ?
Rb1 Na1 Rb1 101.88(2) 18_656 16_556 ?
Rb1 Na1 Rb1 141.00(4) 3_655 16_556 ?
Rb1 Na1 Rb1 108.72(9) 5 16_556 ?
O4 N1 O4 120.000(1) 3_655 14_666 ?
O4 N1 O4 120.000(1) 3_655 . ?
O4 N1 O4 120.000(1) 14_666 . ?
O4 N1 Na1 57.2(2) 3_655 3_655 ?
O4 N1 Na1 62.8(2) 14_666 3_655 ?
O4 N1 Na1 177.2(2) . 3_655 ?
O4 N1 Na1 177.2(2) 3_655 14_666 ?
O4 N1 Na1 57.2(2) 14_666 14_666 ?
O4 N1 Na1 62.8(2) . 14_666 ?
Na1 N1 Na1 120.000(1) 3_655 14_666 ?
O2 C1 O2 120.0 14_556 3 ?
O2 C1 O2 120.0 14_556 . ?
O2 C1 O2 120.0 3 . ?
O2 C1 Rb1 143.14(18) 14_556 16_556 ?
O2 C1 Rb1 66.42(17) 3 16_556 ?
O2 C1 Rb1 66.42(16) . 16_556 ?
O2 C1 Rb1 66.42(16) 14_556 5 ?
O2 C1 Rb1 143.14(18) 3 5 ?
O2 C1 Rb1 66.42(16) . 5 ?
Rb1 C1 Rb1 132.837(6) 16_556 5 ?
O2 C1 Rb1 66.42(17) 14_556 3 ?
O2 C1 Rb1 66.42(17) 3 3 ?
O2 C1 Rb1 143.14(18) . 3 ?
Rb1 C1 Rb1 132.837(6) 16_556 3 ?
Rb1 C1 Rb1 87.722(14) 5 3 ?
O2 C1 Rb1 66.42(17) 14_556 14_556 ?
O2 C1 Rb1 143.14(18) 3 14_556 ?
O2 C1 Rb1 66.42(17) . 14_556 ?
Rb1 C1 Rb1 87.722(14) 16_556 14_556 ?
Rb1 C1 Rb1 73.720(19) 5 14_556 ?
Rb1 C1 Rb1 132.837(6) 3 14_556 ?
O2 C1 Rb1 66.42(16) 14_556 18_556 ?
O2 C1 Rb1 66.42(16) 3 18_556 ?
O2 C1 Rb1 143.14(18) . 18_556 ?
Rb1 C1 Rb1 87.722(14) 16_556 18_556 ?
Rb1 C1 Rb1 132.837(6) 5 18_556 ?
Rb1 C1 Rb1 73.720(19) 3 18_556 ?
Rb1 C1 Rb1 87.722(14) 14_556 18_556 ?
O3 C2 O3 120.0 3_655 5_665 ?
O3 C2 O3 120.0 3_655 . ?
O3 C2 O3 120.0 5_665 . ?
Na1 O1 Rb1 90.06(16) 14_666 . ?
Na1 O1 Rb1 82.80(11) 14_666 3_665 ?
Rb1 O1 Rb1 134.93(5) . 3_665 ?
Na1 O1 Rb1 82.80(11) 14_666 5_665 ?
Rb1 O1 Rb1 134.93(5) . 5_665 ?
Rb1 O1 Rb1 88.36(9) 3_665 5_665 ?
Na1 O1 H1 128.1 14_666 . ?
Rb1 O1 H1 92.7 . . ?
Rb1 O1 H1 126.3 3_665 . ?
Rb1 O1 H1 59.7 5_665 . ?
C1 O2 Na1 180.0(4) . . ?
C1 O2 Rb1 91.67(14) . 16_556 ?
Na1 O2 Rb1 88.33(11) . 16_556 ?
C1 O2 Rb1 91.67(19) . 5 ?
Na1 O2 Rb1 88.33(7) . 5 ?
Rb1 O2 Rb1 176.65(7) 16_556 5 ?
C1 O2 Rb1 91.7(2) . 14_556 ?
Na1 O2 Rb1 88.33(7) . 14_556 ?
Rb1 O2 Rb1 98.18(11) 16_556 14_556 ?
Rb1 O2 Rb1 81.72(8) 5 14_556 ?
C1 O2 Rb1 91.67(14) . . ?
Na1 O2 Rb1 88.33(12) . . ?
Rb1 O2 Rb1 81.72(9) 16_556 . ?
Rb1 O2 Rb1 98.18(11) 5 . ?
Rb1 O2 Rb1 176.65(7) 14_556 . ?
C2 O3 Rb1 128.72(6) . 15 ?
C2 O3 Rb1 128.72(6) . . ?
Rb1 O3 Rb1 102.56(11) 15 . ?
N1 O4 Na1 98.5(3) . . ?
N1 O4 Na1 92.6(2) . 14_666 ?
Na1 O4 Na1 168.88(17) . 14_666 ?
N1 O4 Rb1 136.69(6) . . ?
Na1 O4 Rb1 87.53(12) . . ?
Na1 O4 Rb1 84.35(10) 14_666 . ?
N1 O4 Rb1 136.69(6) . 16_556 ?
Na1 O4 Rb1 87.53(12) . 16_556 ?
Na1 O4 Rb1 84.35(10) 14_666 16_556 ?
Rb1 O4 Rb1 86.13(10) . 16_556 ?
Rb1 Br1 Rb1 180.00(2) 13 . ?
Rb1 Br1 Rb1 90.688(14) 13 17 ?
Rb1 Br1 Rb1 89.312(14) . 17 ?
Rb1 Br1 Rb1 89.312(14) 13 3 ?
Rb1 Br1 Rb1 90.688(14) . 3 ?
Rb1 Br1 Rb1 89.312(14) 17 3 ?
Rb1 Br1 Rb1 90.688(14) 13 15 ?
Rb1 Br1 Rb1 89.312(14) . 15 ?
Rb1 Br1 Rb1 90.688(14) 17 15 ?
Rb1 Br1 Rb1 180.000(19) 3 15 ?
Rb1 Br1 Rb1 89.312(14) 13 5 ?
Rb1 Br1 Rb1 90.688(14) . 5 ?
Rb1 Br1 Rb1 180.000(19) 17 5 ?
Rb1 Br1 Rb1 90.688(14) 3 5 ?
Rb1 Br1 Rb1 89.312(14) 15 5 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O3 Rb1 O1 Na1 130.62(4) 17 . . 14_666 ?
O3 Rb1 O1 Na1 -130.62(4) . . . 14_666 ?
O4 Rb1 O1 Na1 -40.11(7) . . . 14_666 ?
O4 Rb1 O1 Na1 40.11(7) 19 . . 14_666 ?
O2 Rb1 O1 Na1 30.42(12) 3 . . 14_666 ?
O2 Rb1 O1 Na1 -30.42(9) . . . 14_666 ?
Br1 Rb1 O1 Na1 180.0 . . . 14_666 ?
O1 Rb1 O1 Na1 -95.23(9) 3_655 . . 14_666 ?
O1 Rb1 O1 Na1 95.23(9) 5_565 . . 14_666 ?
Na1 Rb1 O1 Na1 57.78(3) 3 . . 14_666 ?
O3 Rb1 O1 Rb1 50.76(15) 17 . . 3_665 ?
O3 Rb1 O1 Rb1 149.52(19) . . . 3_665 ?
O4 Rb1 O1 Rb1 -120.0(2) . . . 3_665 ?
O4 Rb1 O1 Rb1 -39.75(16) 19 . . 3_665 ?
O2 Rb1 O1 Rb1 -49.4(3) 3 . . 3_665 ?
O2 Rb1 O1 Rb1 -110.28(7) . . . 3_665 ?
Br1 Rb1 O1 Rb1 100.14(16) . . . 3_665 ?
O1 Rb1 O1 Rb1 -175.09(8) 3_655 . . 3_665 ?
O1 Rb1 O1 Rb1 15.4(3) 5_565 . . 3_665 ?
Na1 Rb1 O1 Rb1 -79.86(16) 14_666 . . 3_665 ?
Na1 Rb1 O1 Rb1 -22.08(19) 3 . . 3_665 ?
O3 Rb1 O1 Rb1 -149.52(19) 17 . . 5_665 ?
O3 Rb1 O1 Rb1 -50.76(15) . . . 5_665 ?
O4 Rb1 O1 Rb1 39.75(16) . . . 5_665 ?
O4 Rb1 O1 Rb1 120.0(2) 19 . . 5_665 ?
O2 Rb1 O1 Rb1 110.28(11) 3 . . 5_665 ?
O2 Rb1 O1 Rb1 49.4(3) . . . 5_665 ?
Br1 Rb1 O1 Rb1 -100.14(16) . . . 5_665 ?
O1 Rb1 O1 Rb1 -15.4(3) 3_655 . . 5_665 ?
O1 Rb1 O1 Rb1 175.09(8) 5_565 . . 5_665 ?
Na1 Rb1 O1 Rb1 79.86(16) 14_666 . . 5_665 ?
Na1 Rb1 O1 Rb1 137.63(15) 3 . . 5_665 ?
O2 C1 O2 Na1 90(100) 14_556 . . . ?
O2 C1 O2 Na1 -90(100) 3 . . . ?
Rb1 C1 O2 Na1 -131(100) 16_556 . . . ?
Rb1 C1 O2 Na1 49(100) 5 . . . ?
Rb1 C1 O2 Na1 0(100) 3 . . . ?
Rb1 C1 O2 Na1 131(100) 14_556 . . . ?
Rb1 C1 O2 Na1 180(100) 18_556 . . . ?
O2 C1 O2 Rb1 -139.12(17) 14_556 . . 16_556 ?
O2 C1 O2 Rb1 40.9(4) 3 . . 16_556 ?
Rb1 C1 O2 Rb1 180.00(15) 5 . . 16_556 ?
Rb1 C1 O2 Rb1 130.88(17) 3 . . 16_556 ?
Rb1 C1 O2 Rb1 -98.23(12) 14_556 . . 16_556 ?
Rb1 C1 O2 Rb1 -49.1(3) 18_556 . . 16_556 ?
O2 C1 O2 Rb1 40.88(6) 14_556 . . 5 ?
O2 C1 O2 Rb1 -139.1(2) 3 . . 5 ?
Rb1 C1 O2 Rb1 180.00(15) 16_556 . . 5 ?
Rb1 C1 O2 Rb1 -49.1(3) 3 . . 5 ?
Rb1 C1 O2 Rb1 81.77(9) 14_556 . . 5 ?
Rb1 C1 O2 Rb1 130.88(17) 18_556 . . 5 ?
O2 C1 O2 Rb1 -40.88(6) 14_556 . . 14_556 ?
O2 C1 O2 Rb1 139.1(3) 3 . . 14_556 ?
Rb1 C1 O2 Rb1 98.23(12) 16_556 . . 14_556 ?
Rb1 C1 O2 Rb1 -81.77(9) 5 . . 14_556 ?
Rb1 C1 O2 Rb1 -130.88(17) 3 . . 14_556 ?
Rb1 C1 O2 Rb1 49.1(3) 18_556 . . 14_556 ?
O2 C1 O2 Rb1 139.12(16) 14_556 . . . ?
O2 C1 O2 Rb1 -40.9(4) 3 . . . ?
Rb1 C1 O2 Rb1 -81.77(9) 16_556 . . . ?
Rb1 C1 O2 Rb1 98.23(12) 5 . . . ?
Rb1 C1 O2 Rb1 49.1(3) 3 . . . ?
Rb1 C1 O2 Rb1 180.00(14) 14_556 . . . ?
Rb1 C1 O2 Rb1 -130.88(17) 18_556 . . . ?
O1 Na1 O2 C1 180(100) 18_656 . . . ?
O1 Na1 O2 C1 0(100) 3_655 . . . ?
O4 Na1 O2 C1 -90(100) 8 . . . ?
O4 Na1 O2 C1 90(100) . . . . ?
O4 Na1 O2 C1 90(100) 3_655 . . . ?
O4 Na1 O2 C1 -90(100) 21_655 . . . ?
N1 Na1 O2 C1 -90(100) 19_545 . . . ?
Rb1 Na1 O2 C1 180(100) 18_656 . . . ?
Rb1 Na1 O2 C1 0(100) 3_655 . . . ?
Rb1 Na1 O2 C1 -49(100) 5 . . . ?
Rb1 Na1 O2 C1 131(100) 16_556 . . . ?
O1 Na1 O2 Rb1 49.12(7) 18_656 . . 16_556 ?
O1 Na1 O2 Rb1 -130.88(6) 3_655 . . 16_556 ?
O4 Na1 O2 Rb1 139.12(7) 8 . . 16_556 ?
O4 Na1 O2 Rb1 -40.88(7) . . . 16_556 ?
O4 Na1 O2 Rb1 -40.88(16) 3_655 . . 16_556 ?
O4 Na1 O2 Rb1 139.12(7) 21_655 . . 16_556 ?
N1 Na1 O2 Rb1 139.12(4) 19_545 . . 16_556 ?
Rb1 Na1 O2 Rb1 49.12(18) 18_656 . . 16_556 ?
Rb1 Na1 O2 Rb1 -130.88(11) 3_655 . . 16_556 ?
Rb1 Na1 O2 Rb1 180.00(13) 5 . . 16_556 ?
O1 Na1 O2 Rb1 -130.88(6) 18_656 . . 5 ?
O1 Na1 O2 Rb1 49.12(7) 3_655 . . 5 ?
O4 Na1 O2 Rb1 -40.88(7) 8 . . 5 ?
O4 Na1 O2 Rb1 139.12(7) . . . 5 ?
O4 Na1 O2 Rb1 139.12(7) 3_655 . . 5 ?
O4 Na1 O2 Rb1 -40.88(16) 21_655 . . 5 ?
N1 Na1 O2 Rb1 -40.88(10) 19_545 . . 5 ?
Rb1 Na1 O2 Rb1 -130.88(10) 18_656 . . 5 ?
Rb1 Na1 O2 Rb1 49.12(18) 3_655 . . 5 ?
Rb1 Na1 O2 Rb1 180.00(13) 16_556 . . 5 ?
O1 Na1 O2 Rb1 -49.12(7) 18_656 . . 14_556 ?
O1 Na1 O2 Rb1 130.88(6) 3_655 . . 14_556 ?
O4 Na1 O2 Rb1 40.88(6) 8 . . 14_556 ?
O4 Na1 O2 Rb1 -139.12(7) . . . 14_556 ?
O4 Na1 O2 Rb1 -139.12(7) 3_655 . . 14_556 ?
O4 Na1 O2 Rb1 40.88(16) 21_655 . . 14_556 ?
N1 Na1 O2 Rb1 40.88(10) 19_545 . . 14_556 ?
Rb1 Na1 O2 Rb1 -49.12(18) 18_656 . . 14_556 ?
Rb1 Na1 O2 Rb1 130.88(11) 3_655 . . 14_556 ?
Rb1 Na1 O2 Rb1 81.77(8) 5 . . 14_556 ?
Rb1 Na1 O2 Rb1 -98.23(11) 16_556 . . 14_556 ?
O1 Na1 O2 Rb1 130.88(6) 18_656 . . . ?
O1 Na1 O2 Rb1 -49.12(7) 3_655 . . . ?
O4 Na1 O2 Rb1 -139.12(7) 8 . . . ?
O4 Na1 O2 Rb1 40.88(6) . . . . ?
O4 Na1 O2 Rb1 40.88(16) 3_655 . . . ?
O4 Na1 O2 Rb1 -139.12(7) 21_655 . . . ?
N1 Na1 O2 Rb1 -139.12(4) 19_545 . . . ?
Rb1 Na1 O2 Rb1 130.88(11) 18_656 . . . ?
Rb1 Na1 O2 Rb1 -49.12(18) 3_655 . . . ?
Rb1 Na1 O2 Rb1 -98.23(11) 5 . . . ?
Rb1 Na1 O2 Rb1 81.77(8) 16_556 . . . ?
O3 Rb1 O2 C1 -8.2(3) 17 . . . ?
O3 Rb1 O2 C1 -144.95(15) . . . . ?
O4 Rb1 O2 C1 143.1(2) . . . . ?
O4 Rb1 O2 C1 71.72(18) 19 . . . ?
O1 Rb1 O2 C1 133.32(10) . . . . ?
O2 Rb1 O2 C1 20.47(15) 3 . . . ?
Br1 Rb1 O2 C1 -65.66(16) . . . . ?
O1 Rb1 O2 C1 -145.0(2) 3_655 . . . ?
O1 Rb1 O2 C1 7.3(2) 5_565 . . . ?
Na1 Rb1 O2 C1 115.18(16) 14_666 . . . ?
Na1 Rb1 O2 C1 33.03(15) 3 . . . ?
O3 Rb1 O2 Na1 171.82(10) 17 . . . ?
O3 Rb1 O2 Na1 35.05(13) . . . . ?
O4 Rb1 O2 Na1 -36.91(10) . . . . ?
O4 Rb1 O2 Na1 -108.28(12) 19 . . . ?
O1 Rb1 O2 Na1 -46.68(17) . . . . ?
O2 Rb1 O2 Na1 -159.53(16) 3 . . . ?
Br1 Rb1 O2 Na1 114.34(9) . . . . ?
O1 Rb1 O2 Na1 34.96(10) 3_655 . . . ?
O1 Rb1 O2 Na1 -172.70(8) 5_565 . . . ?
Na1 Rb1 O2 Na1 -64.82(9) 14_666 . . . ?
Na1 Rb1 O2 Na1 -146.97(10) 3 . . . ?
O3 Rb1 O2 Rb1 -99.63(17) 17 . . 16_556 ?
O3 Rb1 O2 Rb1 123.60(6) . . . 16_556 ?
O4 Rb1 O2 Rb1 51.64(8) . . . 16_556 ?
O4 Rb1 O2 Rb1 -19.73(9) 19 . . 16_556 ?
O1 Rb1 O2 Rb1 41.88(10) . . . 16_556 ?
O2 Rb1 O2 Rb1 -70.98(7) 3 . . 16_556 ?
Br1 Rb1 O2 Rb1 -157.11(3) . . . 16_556 ?
O1 Rb1 O2 Rb1 123.51(10) 3_655 . . 16_556 ?
O1 Rb1 O2 Rb1 -84.15(6) 5_565 . . 16_556 ?
Na1 Rb1 O2 Rb1 23.73(3) 14_666 . . 16_556 ?
Na1 Rb1 O2 Rb1 -58.42(3) 3 . . 16_556 ?
O3 Rb1 O2 Rb1 83.75(14) 17 . . 5 ?
O3 Rb1 O2 Rb1 -53.02(9) . . . 5 ?
O4 Rb1 O2 Rb1 -124.98(8) . . . 5 ?
O4 Rb1 O2 Rb1 163.65(9) 19 . . 5 ?
O1 Rb1 O2 Rb1 -134.74(11) . . . 5 ?
O2 Rb1 O2 Rb1 112.40(14) 3 . . 5 ?
Br1 Rb1 O2 Rb1 26.27(4) . . . 5 ?
O1 Rb1 O2 Rb1 -53.11(4) 3_655 . . 5 ?
O1 Rb1 O2 Rb1 99.23(9) 5_565 . . 5 ?
Na1 Rb1 O2 Rb1 -152.89(4) 14_666 . . 5 ?
Na1 Rb1 O2 Rb1 124.96(6) 3 . . 5 ?
O3 Rb1 O2 Rb1 172(2) 17 . . 14_556 ?
O3 Rb1 O2 Rb1 35(2) . . . 14_556 ?
O4 Rb1 O2 Rb1 -37(2) . . . 14_556 ?
O4 Rb1 O2 Rb1 -108(2) 19 . . 14_556 ?
O1 Rb1 O2 Rb1 -47(2) . . . 14_556 ?
O2 Rb1 O2 Rb1 -160(2) 3 . . 14_556 ?
Br1 Rb1 O2 Rb1 114(2) . . . 14_556 ?
O1 Rb1 O2 Rb1 35(2) 3_655 . . 14_556 ?
O1 Rb1 O2 Rb1 -173(2) 5_565 . . 14_556 ?
Na1 Rb1 O2 Rb1 -65(2) 14_666 . . 14_556 ?
Na1 Rb1 O2 Rb1 -147(2) 3 . . 14_556 ?
O3 C2 O3 Rb1 -54.25(14) 3_655 . . 15 ?
O3 C2 O3 Rb1 125.76(14) 5_665 . . 15 ?
O3 C2 O3 Rb1 125.76(14) 3_655 . . . ?
O3 C2 O3 Rb1 -54.25(14) 5_665 . . . ?
O3 Rb1 O3 C2 95.97(6) 17 . . . ?
O4 Rb1 O3 C2 -41.09(9) . . . . ?
O4 Rb1 O3 C2 16.22(8) 19 . . . ?
O1 Rb1 O3 C2 28.85(6) . . . . ?
O2 Rb1 O3 C2 -123.45(17) 3 . . . ?
O2 Rb1 O3 C2 -103.49(8) . . . . ?
Br1 Rb1 O3 C2 180.0 . . . . ?
O1 Rb1 O3 C2 -103.39(9) 3_655 . . . ?
O1 Rb1 O3 C2 117.17(9) 5_565 . . . ?
Na1 Rb1 O3 C2 1.64(18) 14_666 . . . ?
Na1 Rb1 O3 C2 88.7(4) 3 . . . ?
O3 Rb1 O3 Rb1 -84.03(6) 17 . . 15 ?
O4 Rb1 O3 Rb1 138.91(9) . . . 15 ?
O4 Rb1 O3 Rb1 -163.78(8) 19 . . 15 ?
O1 Rb1 O3 Rb1 -151.15(6) . . . 15 ?
O2 Rb1 O3 Rb1 56.55(17) 3 . . 15 ?
O2 Rb1 O3 Rb1 76.51(8) . . . 15 ?
Br1 Rb1 O3 Rb1 0.0 . . . 15 ?
O1 Rb1 O3 Rb1 76.61(9) 3_655 . . 15 ?
O1 Rb1 O3 Rb1 -62.83(9) 5_565 . . 15 ?
Na1 Rb1 O3 Rb1 -178.36(2) 14_666 . . 15 ?
Na1 Rb1 O3 Rb1 -91.3(4) 3 . . 15 ?
O4 N1 O4 Na1 0.0 3_655 . . . ?
O4 N1 O4 Na1 180.0 14_666 . . . ?
Na1 N1 O4 Na1 0.0 3_655 . . . ?
Na1 N1 O4 Na1 180.0 14_666 . . . ?
O4 N1 O4 Na1 180.0 3_655 . . 14_666 ?
O4 N1 O4 Na1 0.0 14_666 . . 14_666 ?
Na1 N1 O4 Na1 180.0 3_655 . . 14_666 ?
O4 N1 O4 Rb1 -95.5(3) 3_655 . . . ?
O4 N1 O4 Rb1 84.5(3) 14_666 . . . ?
Na1 N1 O4 Rb1 -95.5(3) 3_655 . . . ?
Na1 N1 O4 Rb1 84.5(3) 14_666 . . . ?
O4 N1 O4 Rb1 95.5(3) 3_655 . . 16_556 ?
O4 N1 O4 Rb1 -84.5(3) 14_666 . . 16_556 ?
Na1 N1 O4 Rb1 95.5(3) 3_655 . . 16_556 ?
Na1 N1 O4 Rb1 -84.5(3) 14_666 . . 16_556 ?
O1 Na1 O4 N1 85.50(14) 18_656 . . . ?
O1 Na1 O4 N1 -85.50(14) 3_655 . . . ?
O2 Na1 O4 N1 180.00(10) . . . . ?
O4 Na1 O4 N1 180.0 8 . . . ?
O4 Na1 O4 N1 0.0 3_655 . . . ?
O4 Na1 O4 N1 0.0 21_655 . . . ?
N1 Na1 O4 N1 0.0 19_545 . . . ?
Rb1 Na1 O4 N1 32.49(3) 18_656 . . . ?
Rb1 Na1 O4 N1 -32.49(3) 3_655 . . . ?
Rb1 Na1 O4 N1 -138.29(10) 5 . . . ?
Rb1 Na1 O4 N1 136.89(5) 16_556 . . . ?
O1 Na1 O4 Na1 -94.50(14) 18_656 . . 14_666 ?
O1 Na1 O4 Na1 94.50(14) 3_655 . . 14_666 ?
O2 Na1 O4 Na1 0.00(10) . . . 14_666 ?
O4 Na1 O4 Na1 0.0 8 . . 14_666 ?
O4 Na1 O4 Na1 180.0 3_655 . . 14_666 ?
O4 Na1 O4 Na1 180.0 21_655 . . 14_666 ?
N1 Na1 O4 Na1 180.0 19_545 . . 14_666 ?
Rb1 Na1 O4 Na1 -147.51(3) 18_656 . . 14_666 ?
Rb1 Na1 O4 Na1 147.51(3) 3_655 . . 14_666 ?
Rb1 Na1 O4 Na1 41.71(10) 5 . . 14_666 ?
Rb1 Na1 O4 Na1 -43.11(5) 16_556 . . 14_666 ?
O1 Na1 O4 Rb1 -137.61(14) 18_656 . . . ?
O1 Na1 O4 Rb1 51.39(15) 3_655 . . . ?
O2 Na1 O4 Rb1 -43.11(11) . . . . ?
O4 Na1 O4 Rb1 -43.11(5) 8 . . . ?
O4 Na1 O4 Rb1 136.89(5) 3_655 . . . ?
O4 Na1 O4 Rb1 136.89(5) 21_655 . . . ?
N1 Na1 O4 Rb1 136.89(5) 19_545 . . . ?
Rb1 Na1 O4 Rb1 169.38(5) 18_656 . . . ?
Rb1 Na1 O4 Rb1 104.40(6) 3_655 . . . ?
Rb1 Na1 O4 Rb1 -1.40(13) 5 . . . ?
Rb1 Na1 O4 Rb1 -86.23(10) 16_556 . . . ?
O1 Na1 O4 Rb1 -51.39(15) 18_656 . . 16_556 ?
O1 Na1 O4 Rb1 137.61(14) 3_655 . . 16_556 ?
O2 Na1 O4 Rb1 43.11(11) . . . 16_556 ?
O4 Na1 O4 Rb1 43.11(5) 8 . . 16_556 ?
O4 Na1 O4 Rb1 -136.89(5) 3_655 . . 16_556 ?
O4 Na1 O4 Rb1 -136.89(5) 21_655 . . 16_556 ?
N1 Na1 O4 Rb1 -136.89(5) 19_545 . . 16_556 ?
Rb1 Na1 O4 Rb1 -104.40(6) 18_656 . . 16_556 ?
Rb1 Na1 O4 Rb1 -169.38(5) 3_655 . . 16_556 ?
Rb1 Na1 O4 Rb1 84.82(9) 5 . . 16_556 ?
O3 Rb1 O4 N1 -66.7(4) 17 . . . ?
O3 Rb1 O4 N1 15.9(4) . . . . ?
O4 Rb1 O4 N1 -127.1(3) 19 . . . ?
O1 Rb1 O4 N1 -54.1(4) . . . . ?
O2 Rb1 O4 N1 167.0(4) 3 . . . ?
O2 Rb1 O4 N1 133.2(4) . . . . ?
Br1 Rb1 O4 N1 89.3(4) . . . . ?
O1 Rb1 O4 N1 64.0(4) 3_655 . . . ?
O1 Rb1 O4 N1 -141.9(3) 5_565 . . . ?
Na1 Rb1 O4 N1 -87.8(4) 14_666 . . . ?
Na1 Rb1 O4 N1 -156.8(4) 3 . . . ?
O3 Rb1 O4 Na1 -166.47(7) 17 . . . ?
O3 Rb1 O4 Na1 -83.91(9) . . . . ?
O4 Rb1 O4 Na1 133.11(8) 19 . . . ?
O1 Rb1 O4 Na1 -153.84(11) . . . . ?
O2 Rb1 O4 Na1 67.23(9) 3 . . . ?
O2 Rb1 O4 Na1 33.43(9) . . . . ?
Br1 Rb1 O4 Na1 -10.51(13) . . . . ?
O1 Rb1 O4 Na1 -35.75(9) 3_655 . . . ?
O1 Rb1 O4 Na1 118.31(13) 5_565 . . . ?
Na1 Rb1 O4 Na1 172.39(11) 14_666 . . . ?
Na1 Rb1 O4 Na1 103.43(12) 3 . . . ?
O3 Rb1 O4 Na1 21.14(11) 17 . . 14_666 ?
O3 Rb1 O4 Na1 103.71(7) . . . 14_666 ?
O4 Rb1 O4 Na1 -39.28(10) 19 . . 14_666 ?
O1 Rb1 O4 Na1 33.77(7) . . . 14_666 ?
O2 Rb1 O4 Na1 -105.15(7) 3 . . 14_666 ?
O2 Rb1 O4 Na1 -138.96(9) . . . 14_666 ?
Br1 Rb1 O4 Na1 177.10(4) . . . 14_666 ?
O1 Rb1 O4 Na1 151.86(10) 3_655 . . 14_666 ?
O1 Rb1 O4 Na1 -54.08(14) 5_565 . . 14_666 ?
Na1 Rb1 O4 Na1 -68.95(10) 3 . . 14_666 ?
O3 Rb1 O4 Rb1 105.84(8) 17 . . 16_556 ?
O3 Rb1 O4 Rb1 -171.60(10) . . . 16_556 ?
O4 Rb1 O4 Rb1 45.42(13) 19 . . 16_556 ?
O1 Rb1 O4 Rb1 118.47(11) . . . 16_556 ?
O2 Rb1 O4 Rb1 -20.46(9) 3 . . 16_556 ?
O2 Rb1 O4 Rb1 -54.26(8) . . . 16_556 ?
Br1 Rb1 O4 Rb1 -98.20(9) . . . 16_556 ?
O1 Rb1 O4 Rb1 -123.44(12) 3_655 . . 16_556 ?
O1 Rb1 O4 Rb1 30.62(18) 5_565 . . 16_556 ?
Na1 Rb1 O4 Rb1 84.70(9) 14_666 . . 16_556 ?
Na1 Rb1 O4 Rb1 15.74(11) 3 . . 16_556 ?
O3 Rb1 Br1 Rb1 0.000(13) 17 . . 13 ?
O3 Rb1 Br1 Rb1 0.000(3) . . . 13 ?
O4 Rb1 Br1 Rb1 0.000(17) . . . 13 ?
O4 Rb1 Br1 Rb1 0.00(3) 19 . . 13 ?
O1 Rb1 Br1 Rb1 0.000(6) . . . 13 ?
O2 Rb1 Br1 Rb1 0.000(9) 3 . . 13 ?
O2 Rb1 Br1 Rb1 0.000(4) . . . 13 ?
O1 Rb1 Br1 Rb1 0.000(3) 3_655 . . 13 ?
O1 Rb1 Br1 Rb1 0.000(14) 5_565 . . 13 ?
Na1 Rb1 Br1 Rb1 0.000(6) 14_666 . . 13 ?
Na1 Rb1 Br1 Rb1 0.000(14) 3 . . 13 ?
O3 Rb1 Br1 Rb1 0.0 17 . . 17 ?
O3 Rb1 Br1 Rb1 -90.696(15) . . . 17 ?
O4 Rb1 Br1 Rb1 -163.66(8) . . . 17 ?
O4 Rb1 Br1 Rb1 72.96(8) 19 . . 17 ?
O1 Rb1 Br1 Rb1 -45.35(13) . . . 17 ?
O2 Rb1 Br1 Rb1 113.66(6) 3 . . 17 ?
O2 Rb1 Br1 Rb1 155.64(3) . . . 17 ?
O1 Rb1 Br1 Rb1 -140.29(6) 3_655 . . 17 ?
O1 Rb1 Br1 Rb1 49.59(6) 5_565 . . 17 ?
Na1 Rb1 Br1 Rb1 -45.348(7) 14_666 . . 17 ?
Na1 Rb1 Br1 Rb1 79.93(4) 3 . . 17 ?
O3 Rb1 Br1 Rb1 -89.304(15) 17 . . 3 ?
O3 Rb1 Br1 Rb1 180.0 . . . 3 ?
O4 Rb1 Br1 Rb1 107.04(8) . . . 3 ?
O4 Rb1 Br1 Rb1 -16.34(8) 19 . . 3 ?
O1 Rb1 Br1 Rb1 -134.65(12) . . . 3 ?
O2 Rb1 Br1 Rb1 24.36(6) 3 . . 3 ?
O2 Rb1 Br1 Rb1 66.34(3) . . . 3 ?
O1 Rb1 Br1 Rb1 130.41(6) 3_655 . . 3 ?
O1 Rb1 Br1 Rb1 -39.71(6) 5_565 . . 3 ?
Na1 Rb1 Br1 Rb1 -134.652(8) 14_666 . . 3 ?
Na1 Rb1 Br1 Rb1 -9.38(4) 3 . . 3 ?
O3 Rb1 Br1 Rb1 90.696(15) 17 . . 15 ?
O3 Rb1 Br1 Rb1 0.0 . . . 15 ?
O4 Rb1 Br1 Rb1 -72.96(8) . . . 15 ?
O4 Rb1 Br1 Rb1 163.66(8) 19 . . 15 ?
O1 Rb1 Br1 Rb1 45.35(13) . . . 15 ?
O2 Rb1 Br1 Rb1 -155.64(6) 3 . . 15 ?
O2 Rb1 Br1 Rb1 -113.66(3) . . . 15 ?
O1 Rb1 Br1 Rb1 -49.59(6) 3_655 . . 15 ?
O1 Rb1 Br1 Rb1 140.29(6) 5_565 . . 15 ?
Na1 Rb1 Br1 Rb1 45.348(8) 14_666 . . 15 ?
Na1 Rb1 Br1 Rb1 170.62(4) 3 . . 15 ?
O3 Rb1 Br1 Rb1 180.0 17 . . 5 ?
O3 Rb1 Br1 Rb1 89.304(15) . . . 5 ?
O4 Rb1 Br1 Rb1 16.34(8) . . . 5 ?
O4 Rb1 Br1 Rb1 -107.04(8) 19 . . 5 ?
O1 Rb1 Br1 Rb1 134.65(13) . . . 5 ?
O2 Rb1 Br1 Rb1 -66.34(6) 3 . . 5 ?
O2 Rb1 Br1 Rb1 -24.36(3) . . . 5 ?
O1 Rb1 Br1 Rb1 39.71(6) 3_655 . . 5 ?
O1 Rb1 Br1 Rb1 -130.41(6) 5_565 . . 5 ?
Na1 Rb1 Br1 Rb1 134.652(7) 14_666 . . 5 ?
Na1 Rb1 Br1 Rb1 -100.07(4) 3 . . 5 ?

_diffrn_measured_fraction_theta_max 0.997
_diffrn_reflns_theta_full        28.28
_diffrn_measured_fraction_theta_full 0.997
_refine_diff_density_max         0.553
_refine_diff_density_min         -0.562
_refine_diff_density_rms         0.099
